13.1 FOUNDRY PRACTICE AND EQUIPMENT
by Chuck Fennell
REFERENCES: Publications of the American Foundrytmen’s Society: “Cast
Metals Handbook,” Alloy Cast Irons Handbook,” “Copper-base Alloys Foundry
Practice,” Foundry Sand Handbook.” “Steel Castings Handbook,” Steel Founders’
Society of America. Current publications of ASM International. Current publica-
tions of the suppliers of nonferrous metals relating to the casting of those metals;
i.e., Aluminum Corp. of America, Reynolds Metal Co., Dow Chemical Co., INCO
Alloys International, Inc., RMI Titanium Co., and Copper Development Assn.
Publications of the International Lead and Zinc Research Organization (ILZRO).
BASIC STEPS IN MAKING SAND CASTINGS
The basic steps involved in making sand castings are:
1. Patternmaking. Patterns are required to make molds. The mold is
made by packing molding sand around the pattern. The mold is usu-
ally made in two parts so that the pattern can be withdrawn. In hori-
zontal molding, the top half is called the cope, and the bottom half is
called the drag. In vertical molding, the leading half of the mold is
called the swing, and the back half is called the ram. When the pattern
is withdrawn from the molding material (sand or other), the imprint of
the pattern provides the cavity when the mold parts are brought
together. The mold cavity, together with any internal cores (see
below) as required, is ultimately filled with molten metal to form the
2. If the casting is to be hollow, additional patterns, referred to as
core boxes, are needed to shape the sand forms, or cores, that are placed
in the mold cavity to form the interior surfaces and sometimes the exter-
nal surfaces as well of the casting. Thus the void between the mold and
core eventually becomes the casting.
3. Molding is the operation necessary to prepare a mold for receiving
the metal. It consists of ramming sand around the pattern placed in a
support, or flask, removing the pattern, setting cores in place, and cre-
ating the gating/feeding system to direct the metal into the mold cavity
created by the pattern, either by cutting it into the mold by hand or by
including it on the pattern, which is most commonly used.
4. Melting and pouring are the processes of preparing molten metal of
the proper composition and temperature and pouring this into the mold
from transfer ladles.
5. Cleaning includes all the operations required to remove the gates
and risers that constitute the gating/feeding system and to remove the
adhering sand, scale, parting fins, and other foreign material that must
be removed before the casting is ready for shipment or other process-
ing. Inspection follows, to check for defects in the casting as well as to
ensure that the casting has the dimensions specified on the drawing
and/or specifications. Inspection for internal defects may be quite
involved, depending on the quality specified for the casting (see
Sec. 5.4). The inspected and accepted casting sometimes is used as is,
but often it is subject to further processing which may include heat
treatment, painting, rust preventive oils, other surface treatment (e.g.,
hot-dip galvanizing), and machining. Final operations may include
electrodeposited plated metals for either cosmetic or operational
Since patterns are the forms for the castings, the casting can be no bet-
ter than the patterns from which it is made. Where close tolerances or
smooth casting finishes are desired, it is particularly important that pat-
terns be carefully designed, constructed, and finished.
Patterns serve a variety of functions, the more important being (1) to
shape the mold cavity to produce castings, (2) to accommodate the char-
acteristics of the metal cast, (3) to provide accurate dimensions, (4) to
provide a means of getting liquid metal into the mold (gating system),
and (5) to provide a means to support cores by using core prints outside
of the casting.
Usual allowances built into the pattern to ensure dimensional accu-
racy include the following: (1) Draft, the taper on the vertical walls of
the casting which is necessary to extract the pattern from the mold with-
out disturbing the mold walls and is also required when making the
core. (2) Shrinkage allowance, a correction to compensate for the solidi-
fication shrinkage of the metal and its contraction during cooling. These
allowances vary with the type of metal and size of casting. Typical
allowances for cast iron are to in/ft; for steel, to in/ft; and
for aluminum, to in/ft. A designer should consult appropriate
references (AFS, “Cast Metals Handbook”; ASM, “Casting Design
Handbook”; “Design of Ferrous Castings”) or the foundry. These
allowances also include a size tolerance for the process so that the
casting is dimensionally correct. (See also Secs. 6.1, 6.3, and 6.4.)
Table 13.1.1 lists additional data for some commonly cast metals.
(3) Machine finish allowance is necessary if machining operations are to
be used so that stock is provided for machining. Tabulated data are
available in the references cited for shrinkage allowances. (4) If a casting
is prone to distortion, a pattern may be intentionally distorted to com-
pensate. This is a distortion allowance.
Patterns vary in complexity, depending on the size and number of
castings required. Loose patterns are single prototypes of the casting and
are used only when a few castings are needed. They are usually con-
structed of wood, but metal, plaster, plastics, urethanes, or other suit-
able material may be used. With advancements in solids modeling
utilizing computers, CAD/CAM systems, and laser technology, rapid
prototyping is possible and lends itself to the manufacture of protype
patterns from a number of materials, including dense wax paper, or via
stereolithographic processes wherein a laser-actuated polymerized plas-
tic becomes the actual pattern or a prototype for a pattern or a series of
patterns. The gating system for feeding the casting is cut into the sand
by hand. Some loose patterns may be split into two parts to facilitate
Gated patterns incorporate a gating system along with the pattern to
eliminate hand cutting.
Match-plate patterns have the cope and drag portions of the pattern
mounted on opposite sides of a wooden or metal plate, and are designed
to speed up the molding process. Gating systems are also usually attached.
These patterns are generally used with some type of molding machine
and are recommended where a large number of castings are required.
Table 13.1.1 Average Linear Shrinkage of Castings
Bar iron, rolled 1:55 Cast iron 1:96 Steel, puddled 1:72
Bell metal 1:65 Gun metal 1:134 Steel, wrought 1:64
Bismuth 1:265 Iron, fine grained 1:72 Tin 1:128
Brass 1:65 Lead 1:92 Zinc, cast 1:624
Bronze 1:63 Steel castings 1:50 8 Cu ϩ 1 Sn (by weight) 1:13
Section_13.qxd 10/05/06 10:32 Page 13-3
13-4 FOUNDRY PRACTICE AND EQUIPMENT
For fairly large castings or where an increase in production rate is
desired, the patterns can be mounted on separate pattern plates, which
are referred to as cope- and drag-pattern plates. They are utilized in hor-
izontal or vertical machines. In horizontal molding machines, the pat-
tern plates may be used on separate machines by different workers, and
then combined into completed molds on the molding floor prior to
pouring. In vertical machines, the pattern plates are used on the same
machine, with the flaskless mold portions pushed out one behind the
other. Vertical machines result in faster production rates and provide an
economic edge in overall casting costs.
Special Patterns and Devices For extremely large castings, skeleton
patterns may be employed. Large molds of a symmetric nature may be
made for forming the sand mold by sweeps, which provide the contour of
the casting through the movement of a template around an axis.
Follow boards are used to support irregularly shaped, loose patterns
which require an irregular parting line between cope and drag. A master
pattern is used as an original to make up a number of similar patterns
that will be used directly in the foundry.
MOLDING PROCESSES AND MATERIALS
(See Table 13.1.2.)
Green Sand Most castings are made in green sand, i.e., sand bonded
with clay or bentonite and properly tempered with water to give it green
strength. Miscellaneous additions may be used for special properties.
This method is adaptable to high production of small- or medium-sized
castings because the mold can be poured immediately after forming, and
the sand can be reused and reprocessed after the casting has solidified.
Dry Sand Molds These molds are made with green sand but are
baked prior to use. The surface is usually given a refractory wash before
baking to prevent erosion and to produce a better surface finish. Some-
what the same effects are obtained if the mold is allowed to air-dry by
leaving it open for a period of time before pouring, or it is skin-dried by
using a torch, infrared lamps, or heating elements directed at the mold
Core molding makes use of assembled cores to construct the mold.
The sand is prepared by mixing with oil, or cereal, forming in core
boxes, and baking. This process is used where the intricacy of the cast-
ing requires it.
Carbon Dioxide Process Molds These molds are made in a man-
ner similar to the green sand process but use sand bonded with sodium
silicate. When the mold is finished, carbon dioxide gas is passed through
the sand to produce a very hard mold with many of the advantages of dry
sand and core molds but requiring no baking.
Floor and Pit Molding When large castings are to be produced,
these may be cast either directly on the floor of the foundry or in pits
in the floor which serve as the flask. Loam molding is a variation of floor
molding in which molding material composed of 50 percent sand and
50 percent clay (approx) is troweled onto a brickwork surface and
brought to dimension by use of patterns, sweeps, or templates.
Shell Molding Sand castings having close dimensional tolerances
and smooth finish can be produced by a process using a synthetic resin
binder. The sand and resin mixture is dumped onto a preheated metal
pattern, which causes the resin in the mixture to set as a thin shell over
the pattern. When the shell has reached the proper thickness, the excess
sand is removed by rotating the pattern to dump out the sand. The
remaining shell is then cured on the pattern and subsequently removed
by stripping it off, using mold release pins which have been properly
spaced and that are mechanically or hydraulically made to protrude
through the pattern. Mating shell halves are bonded, suitably backed by
loose sand or other material, and then ready for metal to be poured.
Current practice using shell molds has produced castings in excess of
1,000 lb, but often the castings weigh much less.
Plaster Molds Plaster or plaster-bonded molds are used for casting
certain aluminum or copper base alloys. Dimensional accuracy and
excellent surface finish make this a useful process for making rubber
tire molds, match plates, etc.
A variation of this method of molding is the Antioch process, using
mixtures of 50 percent silica sand, 40 percent gypsum cement, 8 per-
cent talc, and small amounts of sodium silicate, portland cement, and
magnesium oxide. These dry ingredients are mixed with water and
poured over the pattern. After the mixture is poured, the mold is steam-
treated in an autoclave and then allowed to set in air before drying in an
oven. When the mold has cooled it is ready for pouring. Tolerances of
Ϯ0.005 in (Ϯ0.13 mm) on small castings and Ϯ0.015 in (Ϯ0.38 mm)
on large castings are obtained by this process.
A problem presented by plaster molds lies in inadequate permeability
in the mold material consistent with the desired smooth mold cavity
surface. A closely related process, the Shaw process, provides a solution.
Table 13.1.2 Design and Cost Features of Basic Casting Methods
Design and Shell-mold Permanent- Plaster-mold Investment
cost features Sand casting casting mold casting casting casting Die casting
Choice of materials Wide—ferrous and Wide—except for Restricted—brass, Narrow—brass, Wide—includes Narrow—zinc,
nonferrous low-carbon steels bronze, alumi- bronze, aluminum hard-to-forge and aluminum, brass,
num, some gray machine materials magnesium
Complexity Considerable Moderate Moderate Considerable Greatest Considerable
Size range Great Limited Moderate Moderate Moderate Moderate
Minimum section, in 0.100 0.010 0.010 0.025
Tolerances, in ft* – – Ϫ – 0.003–0.006 –
Surface smoothness, 250–300 150–200 90–125 90–125 90–125 60–125
Design feature Basic casting Considered to be Production eco- Little finishing Best for parts too Most economical
remarks method of good low-cost nomics with sub- required complicated for where applicable
industry casting method stantial quantities other casting
Tool and die costs Low Low to moderate Medium Medium Low to moderate High
Optimum lot size Wide—range from More required than Best when require- From one to sev- Wide—but best Substantial quanti-
few pieces to sand castings ments are in thou- eral hundred for small quantities ties requird
huge quantities sands
Direct labor costs High Moderate Moderate High Very high Low to medium
Finishing costs High Low Low to moderate Low Low Low
Scrap costs Moderate Low Low Low Low Low
* Closer at extra cost.
SOURCE: Cook, “Engineered Castings,” McGraw-Hill.
Section_13.qxd 10/05/06 10:32 Page 13-4
In this process, a refractory aggregate is mixed with a gelling agent and
then poured over the pattern. Initial set of the mixture results in a rub-
bery consistency which allows it to be stripped from the pattern but
which is sufficiently strong to return to the shape it had when on the pat-
tern. The mold is then ignited to burn off the volatile content in the set
gel and baked at very high heat. This last step results in a hard, rigid
mold containing microscopic cracks. The permeability of the completed
mold is enhanced by the presence of the so-called microcrazes, while
the mold retains the high-quality definition of the mold surface.
Two facts are inherent in the nature of sand molds: First, there may
be one or few castings required of a given piece, yet even then an expen-
sive wood pattern is required. Second, the requirement of removal of
the pattern from the mold may involve some very intricate pattern con-
struction. These conditions may be alleviated entirely by the use of the
full mold process, wherein a foamed polystyrene pattern is used. Indeed,
the foamed pattern may be made complete with a gating and runner sys-
tem, and it can incorporate the elimination of draft allowance. In actual
practice, the pattern is left in place in the mold and is instantly vapor-
ized when hot metal is poured. The hot metal which vaporized the foam
fills the mold cavity to the shape occupied previously by the foam pat-
tern. This process is ideal for casting runs of one or a few pieces, but it
can be applied to production quantities by mass-producing the foam
patterns. There is extra expense for the equipment to make the destruc-
tible foam patterns, but often the economics of the total casting process
is quite favorable when compared with resorting to a reusable pattern.
There are particular instances when the extreme complexity of a cast-
ing can make a hand-carved foam pattern financially attractive.
The lost-wax, investment, or precision-casting, process permits the accurate
casting of highly alloyed steels and of nonferrous alloys which are impos-
sible to forge and difficult to machine. The procedure consists of making
an accurate metal die into which the wax or plastic patterns are cast. The
patterns are assembled on a sprue and the assembly sprayed, brushed, or
dipped in a slurry of a fine-grained, highly refractory aggregate, and a pro-
prietary bonding agent composed chiefly of ethyl silicate. This mixture is
then allowed to set. The pattern is coated repeatedly with coarser slurries
until a shell of the aggregate is produced around the pattern. The molds are
allowed to stand until the aggregate has set, after which they are heated in
an oven in an inverted position so that the wax will run out. After the wax
is removed, the molds are baked in a preheat furnace. The molds may then
be supported with loose sand and poured in any conventional manner.
There have been attempts in the past to use frozen mercury as a pattern.
While mercury is a viable pattern material and can be salvaged totally for
reuse, the inherent hazards of handling raw mercury have mitigated against
its continued use to make patterns for investment castings.
All dimensions can be held to a tolerance of Ϯ0.005 in (Ϯ0.13 mm)
with some critical dimensions held to 0.002 in (0.05 mm). Most cast-
ings produced by this process are relatively small.
Faithful reproduction and accurate tolerances can also be attained by
the Shaw process; see above. It combines advantages of dimensional
control of precision molds with the ease of production of conventional
molding. The process makes use of wood or metal patterns and a refrac-
tory mold bonded with an ethyl silicate base material. Since the mold is
rubbery when stripped from the pattern, some back draft is permissible.
In the cement-sand process portland cement is used as the sand binder. A
typical mixture has 11 percent portland cement, 89 percent silica sand, and
water 4 to 7 percent of the total sand and cement. New sand is used for
facing the mold and is backed with ground-up sand which has been rebonded.
Cores are made of the same material. The molds and cores must airdry 24
to 72 h before pouring. The process can be used for either ferrous or non-
ferrous castings. This molding mixture practically eliminates the generation
of gases, forms a hard surface which resists the erosive action of the metal,
and produces castings with good surfaces and accurate dimensions. This
process is seldom used, and then only for specific castings wherein the
preparation of this type of mold outweighs many of its disadvantages.
Permanent-Mold Casting Methods
In the permanent-mold casting method, fluid metal is poured by hand into
metal molds and around metal cores without external pressure. The
molds are mechanically clamped together. Of necessity, the complexity
of the cores must be minimal, inasmuch as they must be withdrawn for
reuse from the finished casting. Likewise, the shape of the molds must
be relatively simple, free of reentrant sections and the like, or else the
mold itself will have to be made in sections, with attendant complexity.
Metals suitable for this type of casting are lead, zinc, aluminum and
magnesium alloys, certain bronzes, and cast iron.
For making iron castings of this type, a number of metal-mold units
are usually mounted on a turntable. The individual operations, such as
coating the mold, placing the cores, closing the mold, pouring, opening
the mold, and ejection of the casting, are performed as each mold passes
certain stations. The molds are preheated before the first casting is
poured. The process produces castings having a dense, fine-grained
structure, free from shrink holes or blowholes. The tool changes are
relatively low, and better surface and closer tolerances are obtained than
with the sand-cast method. It does not maintain tolerances as close or
sections as thin as the die-casting or the plaster-casting methods.
Yellow brasses, which are high in zinc, should not be cast by the
permanent-mold process because the zinc oxide fouls the molds or dies.
The semipermanent mold casting method differs from the permanent
mold casting in that sand cores are used, in some places, instead of
metal cores. The same metals may be cast by this method. This process
is used where cored openings are so irregular in shape, or so undercut,
that metal cores would be too costly or too difficult to handle. The
structure of the metal cast around the sand cores is like that of a sand
casting. The advantages of permanent mold casting in tolerances, den-
sity, appearance, etc., exist only in the section cast against the metal
Graphite molds may be used as short-run permanent molds since they
are easier to machine to shape and can be used for higher-melting point
alloys, e.g., steel. The molds are softer, however, and more susceptible to
erosive damage. Steel railroad wheels may be made in these molds and
can be cast by filling the mold by low-pressure casting methods.
In the slush casting process, the cast metal is allowed partially to
solidify next to the mold walls to produce a thin section, after which the
excess liquid metal is poured out of the permanent mold.
In centrifugal casting the metal is under centrifugal force, developed
by rotating the mold at high speed. This process, used in the manufac-
ture of bronze, steel, and iron castings, has the advantage of producing
sound castings with a minimum of risers. In true centrifugal castings the
metal is poured directly into a mold which is rotated on its own axis.
Obviously, the shapes cast by this method must have external and inter-
nal geometries which are surfaces of revolution. The external cast sur-
face is defined by the internal surface of the water-cooled mold; the
internal surface of the casting results from the effective core of air
which exists while the mold is spun and until the metal solidifies suffi-
ciently to retain its cast shape. Currently, all cast-iron pipe intended for
service under pressure (e.g., water mains) is centrifugally cast. The
process is extended to other metals falling under the rubric of tubular
In pressure casting, for asymmetrical castings which cannot be spun
around their own axes, the mold cavities are arranged around a common
sprue located on the neutral axis of the mold. The molds used in the
centrifugal-casting process may be metal cores or dry sand, depending
on the type of casting and the metal cast.
Die casting machines consist of a basin holding molten metal, a metal-
lic mold or die, and a metal transferring device which automatically
withdraws molten metal from the basin and forces it under pressure into
the die. Two forms of die casting machines are in general use. Lead, tin,
and zinc alloys containing aluminum are handled in piston machines.
Aluminum alloys and pure zinc, or zinc alloys free from aluminum,
rapidly attack the iron in the piston and cylinder and require a different
type of casting machine. The pressures in a piston machine range from
a few hundred to thousands of lb/in2
The gooseneck machine has a cast-iron gooseneck which dips the molten
metal out of the melting pot and transfers it to the die. The pressure is
applied to the molten metal by compressed air after the gooseneck is
brought in contact with the die. This machine, developed primarily for
MOLDING PROCESSES AND MATERIALS 13-5
Section_13.qxd 10/05/06 10:32 Page 13-5
13-6 FOUNDRY PRACTICE AND EQUIPMENT
aluminum alloys, is sometimes used for zinc-aluminum alloys, espe-
cially for large castings, but, owing to the lower pressure, the casting is
likely to be less dense than when made in the piston machine. It is sel-
dom used for magnesium alloys.
In cold chamber machines the molten-metal reservoir is separated from
the casting machine, and just enough metal for one casting is ladled by
hand into a small chamber, from which it is forced into the die under
high pressure. The pressures, quite high, ranging from the low thou-
sands to in excess of 10,000 lb/in2
, are produced by a hydraulic system
connected to the piston in the hot metal chamber. The alloy is kept so
close to its melting temperature that it is in a slushlike condition. The
process is applicable to aluminum alloys, magnesium alloys, zinc
alloys, and even higher-melting-point alloys like brasses and bronzes,
since the pouring well, cylinder, and piston are exposed to the high tem-
perature for only a short time.
All metal mold external pressure castings have close tolerances,
sharp outlines and contours, fine smooth surface, and high rate of pro-
duction, with low labor cost. They have a hard skin and a soft core,
resulting from the rapid chilling effect of the cold metal mold.
The dies usually consist of two blocks of steel, each containing a part
of the cavity, which are locked together while the casting is being made
and drawn apart when it is ready for ejection. One-half of the die (next
to the ejector nozzle) is stationary; the other half moves on a carriage.
The dies are preheated before using and are either air- or water-cooled
to maintain the desired operating temperature. Die life varies with the
alloy and dimensional tolerances required. Retractable and removable
metal cores are used to form internal surfaces. Inserts can be cast into
the piece by placing them on locating pins in the die.
A wide range of sizes and shapes can be made by these processes,
including threaded pieces and gears. Holes can be accurately located.
The process is best suited to large-quantity production.
A historic application of the process was for typesetting machines
such as the linotype. Although now they are obsolescent and rarely
found in service, for a long time the end products of typesetting machines
were a prime example of a high-quality die-cast metal product.
MOLDING EQUIPMENT AND MECHANIZATION
Flasks may be filled with sand by hand shoveling, gravity feed from
overhead hoppers, continuous belt feeding from a bin, sand slingers,
and, for large molds, by an overhead crane equipped with a grab bucket.
Hand ramming is the simplest method of compacting sand. To
increase the rate, pneumatic rammers are used. The method is slow, the
sand is rammed in layers, and it is difficult to gain uniform density.
More uniform results and higher production rates are obtained by
squeezing machines. Hand-operated squeezers were limited to small
molds and are obsolete; air-operated machines permit an increase in the
allowable size of molds as well as in the production rate. These
machines are suitable for shallow molds. Squeezer molding machines
produce greatest sand density at the top of the flask and softest near the
parting line of pattern. Air-operated machines are also applied in vertical
molding processes using flaskless molds. Horizontal impact molding
sends shock waves through the sand to pack the grains tightly.
In jolt molding machines the pattern is placed on a platen attached to
the top of an air cylinder. After the table is raised, a quick-release port
opens, and the piston, platen, and mold drop free against the top of the
cylinder or striking pads. The impact packs the sand. The densities pro-
duced by this machine are greatest next to the parting line of the pattern
and softest near the top of the flask. This procedure can be used for any
flask that can be rammed on a molding machine. As a separate unit, it
is used primarily for medium and large work. Where plain jolt machines
are used on large work, it is usual to ram the top of the flask manually
with an air hammer.
Jolt squeeze machines use both the jolt and the squeeze procedures.
The platen is mounted on two air cylinders: a small cylinder to jolt and
a large one to squeeze the mold. They are widely used for small and
medium work, and with match-plate or gated patterns. Pattern-stripping
devices can be incorporated with jolt or squeezer machines to permit
mechanical removal of the pattern. Pattern removal can also be ac-
complished by using jolt-rockover-draw or jolt-squeeze-rollover-draw
The sand slinger is the most widely applicable type of ramming
machine. It consists of an impeller mounted on the end of a double-jointed
arm which is fed with sand by belt conveyors mounted on the arm. The
impeller rotating at high speed gives sufficient velocity to the sand to ram
it in the mold by impact. The head may be directed to all parts of the flask
manually on the larger machines and may be automatically controlled on
smaller units used for the high-speed production of small molds.
Vibrators are used on all pattern-drawing machines to free the pattern
from the grip of the sand before drawing. Their use reduces mold dam-
age to a minimum when the pattern is removed, and has the additional
advantage of producing castings of more uniform size than can be
secured by hand rapping the pattern. Pattern damage is also kept to a
minimum. Vibrators are usually air-operated, but some electrically
operated types are in use.
Flasks generally consist of two parts: the upper section, called the
cope, and the bottom section, the drag. When more than two parts are
used, the intermediate sections are called cheeks. Flasks are classified as
tight, snap, and slip. Tight flasks are those in which the flask remains
until the metal is poured. Snap flasks are hinged on one corner and have
a locking device on the diagonally opposite corner. In use, these flasks
are removed as soon as the mold is closed. Slip flasks are of solid con-
struction tapered from top to bottom on all four sides so that they can
be removed as soon as the mold is closed. Snap or slip flasks permit the
molder to make any number of molds with one flask. Before pouring
snap- or slip-flask molds, a wood or metal pouring jacket is placed
around the mold and a weight set on the top to keep the cope from
lifting. The cope and drag sections on all flasks are maintained in proper
alignment by flask pins and guides.
Tight flasks can be made in any size and are fabricated of wood,
rolled steel, cast steel, cast iron, magnesium, or aluminum. Wood, alu-
minum, and magnesium are used only for small- and medium-sized
flasks. Snap and slip flasks are made of wood, aluminum, or magne-
sium, and are generally used for molds not over 20 by 20 in (500 mm by
Mechanization of Sand Preparation
In addition to the various types of molding machines, the modern foundry
makes use of a variety of equipment to handle the sand and castings.
Sand Preparation and Handling Sand is prepared in mullers, which
serve to mix the sand, bonding agent, and water. Aerators are used in
conjunction to loosen the sand to make it more amenable to molding.
Sand cutters that operate over a heap on the foundry floor may be used
instead of mullers. Delivery of the sand to the molding floor may be by
means of dump or scoop trucks or by belt conveyors. At the molding
floor the molds may be placed on the floor or delivered by conveyors to
a pouring station.After pouring, the castings are removed from the flasks
and adhering sand at a shakeout station. This may be a mechanically
operated jolting device that shakes the loose sand from flask and casting.
The used sand, in turn, is returned to the storage bins by belt conveyor
or other means. Small castings may be poured by using stackmolding
methods. In this case, each flask has a drag cavity molded in its upper
surface and a cope cavity in its lower surface. These are stacked one on
the other to a suitable height and poured from a common sprue.
There is an almost infinite variety of equipment and methods avail-
able to the foundry, ranging from simple, work-saving devices to com-
pletely mechanized units, including completely automatic molding
machines. Because of this wide selection available, the degree to which
a foundry can be mechanized depends almost entirely on the econom-
ics of the operations, rather than the availability or lack of availability
of a particular piece of equipment.
Molding sand consists of silica grains held together by some bonding
material, usually clay or bentonite.
Section_13.qxd 10/05/06 10:32 Page 13-6
Grain size greatly influences the surface finish of a casting. The proper
grain size is determined by the size of the casting, the quality of surface
required, and the surface tension of the molten metal. The grain size
should be approximately uniform when maximum permeability is desired.
Naturally bonded sands are mixtures of silica and clay as taken from
the pits. Modification may be necessary to produce a satisfactory mix-
ture. This type of sand is used in gray iron, ductile iron, malleable iron,
and nonferrous foundries (except magnesium).
Synthetically bonded sands are produced by combining clay-free silica
sand with clay or bentonite. These sands can be compounded to suit
foundry requirements. They are more uniform than naturally bonded
sands but require more careful mixing and control. Steel foundries, gray
iron and malleable iron foundries, and magnesium foundries use this type
Special additives may be used in addition to the basic sand, clay, and
water. These include cereals, ground pitch, sea coal, gilsonite, fuel oil,
wood flour, silica flour, iron oxide, pearlite, molasses, dextrin, and pro-
prietary materials. These all serve the purpose of altering specific prop-
erties of the sand to give desired results.
The properties of the sand that are of major interest to the foundry
worker are permeability, or the venting power, of the sand; green com-
pressive strength; green shear strength; deformation, or the sand move-
ment under a given load; dry compressive strength; and hot strength, i.e.,
strength at elevated temperatures. Several auxiliary tests are often
made, including moisture content, clay content, and grain-size determi-
The foundry engineer or metallurgist who usually is entrusted with
the control of the sand properties makes the adjustments required to
keep it in good condition.
Facing sands, for giving better surface to the casting, are used for gray
iron, malleable iron, steel, and magnesium castings. The iron sands usu-
ally contain sea coal, a finely ground coal which keeps the sand from
adhering to the casting by generating a gas film when in contact with
the hot metal. Steel facings contain silica flour or other very fine highly
refractory material to form a dense surface which the metal cannot read-
Mold washes are coatings applied to the mold or core surface to
improve the finish of the casting. They are applied either wet or dry. The
usual practice is to brush or spray the wet mold washes and to brush or
rub on the dry ones. Graphite or silica flour mixed with clay and
molasses water is frequently used. The washes are mixed usually with
waterbase or alcohol-base solvent solutions that require oven drying
time, during which not only does the wash set, but also the excess mois-
ture is removed from the washed coating.
Core Sands and Core Binders
Green sand cores are made from standard molding-sand mixtures, some-
times strengthened by adding a binder, such as dextrin, which hardens
the surface. Cores of this type are very fragile and are usually made
with an arbor or wires on the inside to facilitate handling. Their col-
lapsibility is useful to prevent hot tearing of the casting.
Dry sand cores are made from silica sand and a binder (usually oil)
which hardens under the action of heat. The amount of oil used should
be the minimum which will produce the necessary core strength.
Core binders are either organic, such as core oil, which are destroyed
under heat, or inorganic, which are not destroyed.
Organic Binders The main organic binder is core oil. Pure linseed
oil is used extensively as one of the basic ingredients in blended-oil core
binders. These consist primarily of linseed oil, resin, and a thinner, such
as high-grade kerosene. They have good wetting properties, good work-
ability, and better oxidation characteristics than straight linseed oil.
Corn flour produces good green strength and dry strength when used
in conjunction with oil. Cores made with this binder are quick drying in
the oven and burn out rapidly and completely in the mold.
Dextrin produces a hard surface and weak center because of the
migration of dextrin and water to the surface. Used with oil, it produces
a hard smooth surface but does not produce a green bond as good as that
with corn flour.
Commercial protein binders, such as gelatin, casein, and glues,
improve flowability of the sand, have high binding power, rapid drying,
fair resistance to moisture, and low burning-out point, with only a small
volume of gas evolved on burning. They are used where high collapsi-
bility of the core is essential.
Other binders include paper-mill by-products, which absorb moisture
readily, have high dry strength, low green strength, high gas ratio, and
high binding power for clay materials.
Coal tar pitch and petroleum pitch flow with heat and freeze around the
grains on cooling. These compounds have low moisture absorption
rates and are used extensively for large iron cores. They can be used
effectively with impure sands.
Wood and gum rosin, plastic resins, and rosin by-products are used to pro-
duce collapsibility in cores. They must be well ground. They tend to cake
in hot weather, and large amounts are required to get desired strength.
Plastics of the urea- and phenol-formaldehyde groups and furan resins
are being used for core binders. They have the advantage of low-
temperature baking, collapse readily, and produce only small amounts of
gas. These can be used in dielectric baking ovens or in the shell molding,
hot box, or air setting processes for making cores.
Inorganic binders include fire clay, southern bentonite, western ben-
tonite, and iron oxide.
Cores can also be made by mixing sand with sodium silicate. When
this mixture is in the core box, it is infiltrated with CO2, which causes the
core to harden. This is called the CO2 process.
Cores are made by the methods employed for sand molds. In addition,
core blowers and extrusion machines are used.
Core blowers force sand into the core box by compressed air at about
. They can be used for making all types of small- and medium-
sized cores. The cores produced are very uniform, and high production
rates are achieved.
Screw feed machines are used largely for plain cylindrical cores of uni-
form cross section. The core sand is extruded through a die onto a core
plate. The use of these machines is limited to the production of stock
cores, which are cut to the desired length after baking.
Core Ovens Core oven walls are constructed of inner and outer
layers of sheet metal separated by rock wool or Fiberglas insulation and
with interlocked joints. Combustion chambers are refractory-lined, and
the hot gases are circulated by fans. They are designed for operating at
temperatures suitable for the constituents in the core body. Time at bak-
ing temperatures will, likewise, vary with the composition of the core.
Core driers are light skeleton cast iron or aluminum boxes, the inter-
nal shape of which conforms closely to the cope portion of the core.
They are used to support, during baking, cores which cannot be placed
on a flat plate.
Chaplets are metallic pieces inserted into the mold cavity which sup-
port the core. Long unsupported cores will be subject to flotation force
as the molten metal fills the mold and may break if the resulting flexural
stresses are excessive. Likewise, the liquid forces imposed on cores as
metal flows through the mold cavity may cause cores to shift. The chap-
lets interposed within the mold cavity are placed to alleviate these con-
ditions. They are generally made of the same material as that being cast;
they melt and blend with the metal as cast, and they remain solid long
enough for the liquid forces to equilibrate through the mold cavity.
In general, the types of alloys that can be produced as wrought metals
can also be prepared as castings. Certain alloys, however, cannot be
forged or rolled and can only be used as cast.
Steel Castings (See Sec. 6.3.) Steel castings may be classified as:
1. Low carbon (C Ͻ 0.20 percent). These are relatively soft and not
2. Medium carbon (0.20 percent Ͻ C Ͻ 0.50 percent). These castings
are somewhat harder and amenable to strengthening by heat treatment.
CASTING ALLOYS 13-7
Section_13.qxd 10/05/06 10:32 Page 13-7
13-8 FOUNDRY PRACTICE AND EQUIPMENT
3. High carbon (C Ͼ 0.50 percent). These steels are used where max-
imum hardness and wear resistance are desired.
In addition to the classification based on carbon content, which deter-
mines the maximum hardness obtainable in steel, the castings can be
also classified as low alloy content (Յ 8 percent) or high alloy content
(Ͼ 8 percent).
Low-alloy steels behave essentially as plain carbon steels but have a
higher hardenability, which is a measure of ability to be hardened by
heat treatment. High-alloy steels are designed to produce some specific
property, like corrosion resistance, heat resistance, wear resistance, or
some other special property.
Malleable Iron Castings The carbon content of malleable iron
ranges from about 2.00 to 2.80 percent and may reach as high as
3.30 percent if the iron is melted in a cupola. Silicon ranging from 0.90 to
1.80 percent is an additional alloying element required to aid the
annealing of the iron. As cast, this iron is hard and brittle and is rendered
soft and malleable by a long heat-treating or annealing cycle. (See also
Gray Iron Castings Gray iron is an alloy of iron, carbon, and silicon,
containing a higher percentage of these last two elements than found in
malleable iron. Much of the carbon is present in the elemental form as
graphite. Other elements present include manganese, phosphorus, and
sulfur. Because the properties are controlled by proper proportioning of
the carbon and silicon and by the cooling rate of the casting, it is usually
sold on the basis of specified properties rather than composition. The car-
bon content will usually range between 3.00 and 4.00 percent and the sil-
icon will be between 1.00 and 3.00 percent, the higher values of carbon
being used with the lower silicon values (usually), and vice versa. As evi-
dence of the fact that gray iron should not be considered as a material
having a single set of properties, theASTM andAFS codify gray cast iron
in several classes, with accompanying ranges of tensile strengths avail-
able. The high strengths are obtained by proper adjustment of the carbon
and silicon contents or by alloying. (See also Sec. 6.3.)
An important variation of gray iron is nodular iron, or ductile iron, in
which the graphite appears as nodules rather than as flakes. This iron is
prepared by treating the metal in the ladle with additives that usually
include magnesium in alloy form. Nodular iron can exceed 100,000
) as cast and is much more ductile than gray iron,
measuring about 2 to 5 percent elongation at these higher strengths, and
even higher percentages if the strength is lower. (See Sec. 6.3.)
Aluminum-Base Castings Aluminum is alloyed with copper, sili-
con, magnesium, zinc, nickel, and other elements to produce a wide
variety of casting alloys having specific characteristics of foundry prop-
erties, mechanical properties, machinability, and/or corrosion resis-
tance. Alloys are produced for use in sand casting, permanent mold
casting, or die casting. Some alloys are heat-treatable using solution and
age-hardening treatments. (See also Sec. 6.4.)
Copper-Base Alloys The alloying elements used with copper
include zinc (brasses), tin (bronzes), nickel (nickel bronze), aluminum
(aluminum bronze), silicon (silicon bronze), and beryllium (beryllium
bronze). The brasses and tin bronzes may contain lead for machinability.
Various combinations of zinc and tin, or of tin or zinc with other ele-
ments, are also available. With the exception of some of the aluminum
bronzes and beryllium bronze, most of the copper-base alloys cannot be
hardened by heat treatment. (See also Sec. 6.4.)
Special Casting Alloys Other metals cast in the foundry include
magnesium-base alloys for light weight, nickel-base alloys for high-
temperature applications, titanium-base alloys for strength-to-weight
ratio, etc. The magnesium-base alloys require special precautions dur-
ing melting and pouring to avoid burning. (See Sec. 6.4.)
MELTING AND HEAT TREATING FURNACES
There are several types of melting furnaces used in conjunction with
metal casting. Foundry furnaces used in melting practice for ferrous
castings are predominantly electric arc (direct and indirect), induction,
and crucible for small operations. For cast iron, cupolas are still emp-
loyed, although in ever-decreasing quantities. The previous widespread
use of open-hearth furnaces is now relegated to isolated foundries and
is essentially obsolete. In general, ferrous foundries’melting practice has
become based largely on electric-powered furnaces. Duplexing operations
are still employed, usually in the form of cupola/induction furnace, or
cupola/electric arc furnace.
In nonferrous foundries, electric arc, induction, and crucible furnaces
predominate. There are some residual installations which use air fur-
naces, but they are obsolete and found only in some of the older, small
foundries which cater to unique clients.
Vacuum melting and metal refining were fostered by the need for
extremely pure metals for high-temperature, high-strength applications
(e.g., gas-turbine blades). Vacuum melting is accomplished in a furnace
located in an evacuated chamber; the source of heat is most often an
electric arc and sometimes induction coils. Gases entrained in the melt
are removed, the absence of air prevents oxidation of the base metals,
and a high degree of metal purity is retained in the molten metal and in
the casting ultimately made from that vacuum-melted metal. The mold
is also enclosed in the same evacuated chamber.
The vacuum melting and casting process is very expensive because
of the nature of the equipment required, and quantities of metal handled
are relatively small. The economics of the overall process are justified
by the design requirements for highest-quality castings for ultimately
very demanding service.
Annealing and heat-treating furnaces used to process castings are the
type usually found in industrial practice. (See Secs. 7.3. and 7.5.)
CLEANING AND INSPECTION
Tumbling barrels consist of a power-driven drum in which the castings
are tumbled in contact with hard iron stars or balls. Their impact
removes the sand and scale.
In air-blast cleaning units, compressed air forces silica sand or chilled
iron shot into violent contact with the castings, which are tumbled in a
barrel, rotated on a table, or passed between multiple orifices on a con-
veyor. Large rooms are sometimes utilized, with an operator directing
the nozzle. These machines are equipped with hoppers and elevators to
return the sand or shot to the magazine. Dust-collecting systems are
In centrifugal-blast cleaning units, a rotating impeller is used to impart
the necessary velocity to the chilled iron shot or abrasive grit. The veloc-
ities are not so high as with air, but the volume of abrasive is much
greater. The construction is otherwise similar to the air blast machine.
Water in large volume at pressures of 250 to 600 lb/in2
is used to
remove sand and cores from medium and large castings.
High-pressure water and sand cleaning (Hydroblast) employs high pres-
sure water mixed with molding sand which has been washed off the
casting. A sand classifier is incorporated in the sand reclamation
Pneumatic chipping hammers may be used to clean large castings
where the sand is badly burned on and for deep pockets.
Removal of Gates and Risers and Finishing Castings The follow-
ing tabulation shows the most generally used methods for removing
gates and risers (marked R) and for finishing (marked F).
Steel Oxyacetylene (R) hand hammer or sledge (R), grinders (F),
chipping hammer, (F), and machining (F).
Cast iron Chipping hammer (R, F), hand hammer or sledge (R), abra-
sive cutoff (R), power saw (R), and grinders (F).
Malleable iron Hand hammer or sledge (R), grinders (F), shear (F),
and machining (F).
Brass and bronze Chipping hammer (R, F), shear (R, F), hand ham-
mer or sledge (R), abrasive cutoff (R), power saw (R), belt sanders (F),
grinders (F), and machining (F).
Aluminum Chipping hammer (R), shear (R), hand hammer or sledge
(R), power saw (R), grinders (F), and belt sander (F).
Magnesium Band saw (R), machining (F), and flexible-shaft
machines with steel burr cutters (F).
Section_13.qxd 10/05/06 10:32 Page 13-8
(See Sec. 5.4.)
Castings are inspected for dimensional accuracy, hardness, surface fin-
ish, physical properties, internal soundness, and cracks. For hardness and
for physical properties, see Sec. 6.
Internal soundness is checked by cutting or breaking up pilot castings
or by nondestructive testing using X-ray, gamma ray, etc.
Destructive testing tells only the condition of the piece tested and does
not ensure that other pieces not tested will be sound. It is the most com-
monly used procedure at the present time.
X-ray, gamma ray, and other methods have made possible the nonde-
structive checking of castings to determine internal soundness on all
castings produced. Shrinks, cracks, tears, and gas holes can be deter-
mined and repairs made before the castings are shipped.
Magnetic powder tests (Magnaflux) are used to locate structural dis-
continuities in iron and steel except austenitic steels, but they are not
applicable to most nonferrous metals or their alloys. The method is
most useful for the location of surface discontinuities, but it may indi-
cate subsurface defects if the magnetizing force is sufficient to produce
a leakage field at the surface.
In this test a magnetic flux is induced in ferromagnetic material. Any
abrupt discontinuity in its path results in a local flux leakage field. If
finely divided particles of ferromagnetic material are brought into the
vicinity, they offer a low reluctance path to the leakage field and take a
position that outlines approximately its effective boundaries. The cast-
ing to be inspected is magnetized and its surface dusted with the mag-
netic powder. A low velocity air stream blows the excess powder off and
leaves the defect outlined by the powder particles. The powder may be
applied while the magnetizing current is flowing (continuous method)
or after the current is off (residual method). It may be applied dry or sus-
pended in a light petroleum distillate similar to kerosene. Expert inter-
pretation of the tests is necessary.
Design for the best utilization of metal in the cast form requires a knowl-
edge of metal solidification characteristics, foundry practices, and the
metallurgy of the metal being used. Metals exhibit certain peculiarities in
the formation of solid metal during freezing and also undergo shrinkage
in the liquid state during the freezing process and after freezing, and the
casting must be designed to take these factors into consideration.
Knowledge concerning the freezing process will also be of assistance in
determining the fluidity of the metal, its resistance to hot tearing, and its
tendency to evolve dissolved gases. For economy in production, casting
design should take into consideration those factors in molding and coring
that will lead to the simplest procedures. Elimination of expensive cores,
irregular parting lines, and deep drafts in the casting can often be accom-
plished with a slight modification of the original design. Combination of
the foregoing factors with the selection of the right metal for the job is
important in casting design. Consultation between the design engineer
and personnel at the foundry will result in well-designed castings and
cost-effective foundry procedures. Initial guidance may be had from the
several references cited and from updated professional literature, which
abounds in the technical journals. Trade literature, as represented by the
publications issued by the various generic associations, will be useful in
assessing potential problems with specific casting designs. Generally,
time is well spent in these endeavors before an actual design concept is
reduced to a set of dimensional drawings and/or specifications.
13.2 PLASTIC WORKING OF METALS
by Rajiv Shivpuri
(See also Secs. 5 and 6.)
REFERENCES: Crane,“Plastic Working of Metals and Power Press Operations,”
Wiley. Woodworth, “Punches, Dies and Tools for Manufacturing in Presses,”
Henley. Jones, “Die Design and Die Making Practice,” Industrial Press. Stanley,
“Punches and Dies,” McGraw-Hill. DeGarmo, “Materials and Processes in
Manufacturing,” Macmillan. “Modern Plastics Encyclopedia and Engineers
Handbook,” Plastics Catalogue Corp., New York. “The Tool Engineers Hand-
book,” McGraw-Hill. Bridgman, “Large Plastic Flow and Fracture,” McGraw-
Hill. “Cold Working of Metals,” ASM. Pearson, “The Extrusion of Metals,” Wiley.
Yieldable structural forces between the particles composing a material to
be worked are the key to its behavior. Simple internal structures contain
only a single element, as pure copper, silver, or iron. Relatively more dif-
ficult to work are the solid solutions in which one element tends to dis-
tribute uniformly in the structural pattern of another. Thus silver and gold
form a continuous series of solid-solution alloys as their proportions vary.
Next are alloys in which strongly bonded molecular groups dispersed
through or along the grain boundaries of softer metals offer increasing
resistance to working, as does iron carbide (Fe3C) in solution in iron.
Bonding forces are supplied by electric fields characteristic of indi-
vidual atoms. These forces in turn are subject to modification by tem-
perature as energy is added, increasing electron activity.
The particles which constitute an atom are so small that most of its
volume is empty space. For a similar energy state, there is some rough
uniformity in the outside size of atoms. In general, therefore, the more
complex elements have their larger number of particles more densely
packed and so are heavier. For each element, the energy pattern of its
electric charges in motion determines the field characteristics of that
atom and which of the orderly arrangements it will seek to assume with
relation to others like it in the orderly crystalline form.
Space lattice is the term used to describe the orderly arrangement of
rows and layers of atoms in the crystalline form. This orderly state is
also described as balanced, unstrained, or annealed. The working or
deforming of materials distorts the orderly arrangement, unbalancing
the forces between atoms. Cubic patterns or space lattices characterize
the more ductile or workable materials. Hexagonal and more complex
patterns tend to be more brittle or more rigid. Flaws, irregularities, or
distortions, with corresponding unbalanced strains among adjacent
atoms, may occur in the pattern or along grain boundaries. Slip-plane
movements in working to new shapes tend to slide the once orderly lay-
ers of atoms within the grain-boundary limitations of individual crys-
tals. Such sliding movement tends to take place at 45Њ to the direction
of the applied load because much higher stresses are required to pull
atoms directly apart or to push them straight together.
Chemical combinations, in liquid or solid solutions, or molecular com-
pounds depend upon relative field patterns of elements or upon actual
displacement of one or more electrons from the outer orbit of a donor
element to the outer orbit of a receptor element. Thus the molecules of
hard iron carbide, Fe3C, may be held in solid solution in soft pure iron
(ferrite) in increasing proportions up to 0.83 percent of carbon in iron,
which is described as pearlite. Zinc may occupy solid-solution positions
in the copper space lattice up to about 45 percent, the range of the duc-
tile red and yellow brasses.
Thermal Changes Adding heat (energy) increases electron activity
and therefore also the mobility of the atom. Probability of brittle failure at
low temperatures usually becomes less as temperature increases.
Transition temperatures from one state to another differ for different
Section_13.qxd 10/05/06 10:32 Page 13-9
13-10 PLASTIC WORKING OF METALS
elements. Thermal transitions therefore become more complex as such
differing elements are combined in alloys and compounds. As tempera-
tures rise, a stress-relieving range is reached at which the most severely
strained atoms are able to ease themselves around into less strained posi-
tions. At somewhat higher temperatures, annealing or recrystallization of
worked or distorted structure takes place. Old grain boundaries disappear
and small new grains begin to grow, aligning nearby atoms into their
orderly lattice pattern. The more severely the material has been worked,
the lower is the temperature at which recrystallization begins. Grain
growth is more rapid at higher temperatures. In working materials above
their recrystallization range, as in forging, the relief of interatomic strains
becomes more nearly spontaneous as the temperature is increased. Creep
takes place when materials are under some stress above the recrystalliza-
tion range, and the thermal mobility permits individual atoms to ease
around to relieve that stress with an accompanying gradual change of
shape. Thus a wax candle droops due to gravity on a hot day. Lead, which
recrystallizes below room temperature, will creep when used for roofing
or spouting. Steels in rockets and jet engines begin to creep around 1,300
to 1,500ЊF (704 to 815ЊC). Creep is more rapid as the temperature rises
farther above the recrystallization range.
Plasticity is that property of materials which commends them to the
mass-production techniques of pressure-forming desired shapes. It is
understood more easily if several types of plasticity are considered.
Crystoplastic describes materials, notably metals, which can be worked
in the stable crystalling state, below the recrystallization range. Metals
which crystallize in the cubic patterns have a wider plastic range than
those of hexagonal pattern. Alloying narrows the range and increases the
resistance to working. Tensile or compressive testing of an annealed spec-
imen can be used to show the plastic range which lies between the initial
yield point and the point of ultimate tensile or compressive failure.
The plastic range, as of an annealed metal, is illustrated in Fig. 13.2.1.
Changing values of true stress are determined by dividing the applied load
at any instant by the cross-section area at that instant. As material is
worked, a progressive increase in elastic limit and yield point registers the
slip-plane movement or work hardening which has taken place and the
consequent reduction in residual plasticity. This changing yield point or
resistance, shown in Fig. 13.2.1, is divided roughly into three characteristic
ranges. The contour of the lower range can be varied by nonuniformity of
grain sizes or by small displacements resulting from prior direction of
working. Random large, soft grains yield locally under slight displace-
ment, with resulting surface markings, described as orange peel, alligator
skin, or stretcher strain markings. These can be prevented by preparatory
roller leveling, which gives protection in the case of steel for perhaps a day,
or by a 3 to 5 percent temper pass of cold-rolling, which may stress relieve
in perhaps 3 months, permitting recurrent trouble. The middle range cov-
ers most drawing and forming operations. Its upper limit is the point of
normal tensile failure. The upper range requires that metal be worked
primarily in compression to inhibit the start of tensile fracture. Severe
extrusion, spring-temper rolling, and music-wire drawing use this range.
Dispersion hardening of metal alloys by heat treatment (see Fig.
13.2.2) reduces the plastic range and increases the resistance to work
hardening. Figure 13.2.2 also shows the common methods of plotting
change of true stress against percentage of reduction—e.g., reduction of
thickness in rolling or compressive working, of area in wire drawing,
ironing, or tensile testing, or of diameter in cup drawing or reducing
operations—and against true strain, which is the natural logarithm of
change of area, for convenience in higher mathematics.
Fig. 13.2.1 Three ranges of crystoplastic work hardening of a low-carbon steel.
(ASME, 1954, W. S. Wagner, E. W. Bliss Co.)
Fig. 13.2.2 High-range plasticity (dotted) of an SAE 4140 steel, showing the
effect of dispersion hardening. Two plotting methods. (ASME, 1958, Crane and
Wagner, E. W. Bliss Co.)
For metals, thermoplastic working is usually described as hot working,
except for tin and lead, which recrystallize below room temperature.
Hot-worked samples may be etched to show flow lines, which are usually
made up of old-grain boundaries. Where these show, recrystallization
has not yet taken place, and some work hardening is retained to improve
physical properties. Zinc and magnesium, which are typical of the
hexagonal-structure metals, take only small amounts of cold working but
can be drawn or otherwise worked severely at rather moderate tempera-
tures [Zn, 200 to 400ЊF (90 to 200ЊC); Mg, 500 to 700ЊF (260 to
400ЊC)]. Note that, although hexagonal-pattern metals are less easily
worked than cubic-pattern metals, they are for that same reason struc-
turally more rigid for a similar relative weight. Advantageous forging
temperatures change with alloy composition: copper, 1,800 to 1,900ЊF
(980 to 1,040ЊC); red brass, Cu 70, Zn 30, 1,600 to 1,700ЊF (870 to
930ЊC); yellow brass, Cu 60, Zn 40, 1,200 to 1,500ЊF (650 to 815ЊC).
See Sec. 6 for general physical properties of metals.
Substantially pure iron shows an increasing elastic limit and decreas-
ing plasticity with increasing amounts of work hardening by cold-rolling.
The rate at which such work hardening takes place is greatly increased,
and the remaining plasticity reduced, as alloying becomes more complex.
In steels, the mechanical working range is conventionally divided into
cold, warm, and hot working. Figure 13.2.3 is a plot of flow stress, limit
strain, scale factor, and dimensional error for different values of forging
temperature and for two different strain rates. The flow stress is the resis-
tance to deformation. As the temperature rises from room temperature
to 2,072ЊF (1,100ЊC), the flow stress decreases first gradually and then
rapidly to about 25 percent of its value [cold working 114 ksi (786
MPa) and hot working 28 ksi (193 MPa) at a strain of 0.5 and strain rate
of 40 per second].
One measure of workability is the strain limit. As the temperature rises,
the strain limit for the 70-in (inиs) strain rate (typical of mechanical
Section_13.qxd 10/05/06 10:32 Page 13-10
PLASTIC WORKING TECHNIQUES 13-11
press forging) decreases slightly up to 500ЊC (932ЊF), rises until 750ЊC
(1,382ЊF), drops rapidly at 800ЊC (1,472ЊF) (often called blue brittleness),
and beyond 850ЊC (1,562ЊF) increases rapidly to hot forging temperature
of 1,100ЊC (2,012ЊF). Therefore, substantial advantages of low material
resistance (low tool pressures and press loads) and excellent workability
(large flow without material failure) can be realized in the hot-working
range. Hot-working temperatures, however, also mean poor dimensional
tolerance (total dimensional error), poor surface finish, and material loss
due to scale buildup. Forging temperatures above 1,300ЊC (2,372ЊF) can
lead to hot shortness manifested by melting at the grain boundaries.
MATERIAL RESPONSE IN METAL FORMING
The deformation conditions in metalworking processes span a range of
deformation parameters, including strain and strain rates (Fig. 13.2.4) that
are much higher than those encountered in conventional testing methods
(Fig. 13.2.5). In machining, the strains are high and the strain rates can
/s, while in explosive forming, strains are small at high strain
rates providing extremely small response times. Forging and extrusion
cover a wide range of strains and strain rates. Sheet forming carried out
as small strains and strain rates differs from superplastic forming at
extremely low strain rates but high strains. Consequently, different meth-
ods have been developed to test material response for different ranges of
deformation parameters, i.e., strain and strain rate (Fig. 13.2.5).
PLASTIC WORKING TECHNIQUES
In the metalworking operations, as distinguished from metal cutting,
material is forced to move into new shapes by plastic flow. Hot-working
is carried on above the recovery temperature, and spontaneous recovery,
or annealing, occurs about as fast as the properties of the material are
altered by the deformation. This process is limited by the chilling of the
material in the tools, scaling of the material, and the life of the tools at
the required temperatures. Cold-working is carried on at room tempera-
ture and may be applied to most of the common metals. Since, in most
cases, no recovery occurs at this temperature, the properties of the metal
are altered in the direction of increasing strength and brittleness
throughout the working process, and there is consequently a limit to
which cold-working may be carried without danger of fracture.
A convenient way of representing the action of the common metals
when cold-worked consists of plotting the actual stress in the material
against the percentage reduction in thickness. Within the accuracy
required for shop use, the relationship is linear, as in Fig. 13.2.6. The
lower limit of stress shown is the yield point at the softest temper, or
anneal, commercially available, and the upper limit is the limit of ten-
sile action, or the stress at which fracture, rather than flow, occurs. This
latter value does not correspond to the commercially quoted “tensile
strength” of the metal, but rather to the “true tensile strength,” which is
the stress that exists at the reduced section of a tensile specimen at frac-
ture and which is higher than the nominal value in inverse proportion to
the reduction of area of the material.
As an example of the construction and use of the cold-working plots
shown in Fig. 13.2.6, the action of a very-low-carbon deep-drawing
steel has been shown in Fig. 13.2.7. Starting with the annealed material
with a yield point of 35,000 lb/in2
), the steel was drawn
to successive reductions of thickness up to about 58 percent, and the
Fig. 13.2.3 Effect of forging temperature on forgeability and material properties. Material: AISI 1015 steel. f ϭ strain
rate; f* ϭ limiting strain; sf ϭ flow stress; Stot ϭ dimensional error; FeL ϭ scale loss. (K. Lange, “Handbook of Metal
Forming,” McGraw-Hill, 1985.)
0.01 0.1 1.0 10
Fig. 13.2.4 Range of deformation parameters for various metalworking
processes. (Source: P. F. Bariani, S. Bruschi, and T. Dal Negro, Enhancing
Performances of SHPB for Determination of Flow Curves, Annals of the CIRP, 50,
no. 1, pp. 153–156.)
Section_13.qxd 10/05/06 10:32 Page 13-11
13-12 PLASTIC WORKING OF METALS
corresponding stresses plotted as the heavy straight line. The entire
graph was then extrapolated to 100 percent reduction, giving the modu-
lus of strain hardening as indicated, and to zero stress so that all materi-
als might be plotted on the same graph. Lines of equal reduction are
slanting lines through the point marking the modulus of strain harden-
ing at theoretical 100 percent reduction. Starting at any initial condition
of previous cold work on the heavy line, a percentage reduction from
this condition will be indicated by a horizontal traverse to the slanting
reduction line of corresponding magnitude and the resulting increase in
stress by the vertical traverse from this point to the heavy line.
The traverse shown involved three draws from the annealed condition
of 30, 25, and 15 percent each, and resulting stresses of 53,000, 63,000,
and 68,000 lb/in2
(365, 434, and 469 MN/m2
). After the initial 30 percent
reduction, the next 25 percent uses (1.00 Ϫ 0.30) ϫ 0.25, or 17.5 percent
more of the cold-working range; the next 15 percent reduction uses
(1.00 Ϫ 0.30 Ϫ 0.175) ϫ 0.15, or about 8 percent of the original range,
totaling 30 ϩ 17.5 ϩ 8 ϭ 55.5 percent. This may be compared with
the test value percent reduction in area for the particular material. The
same result might have been obtained, die operation permitting, by a
single reduction of 55 percent, as shown. Any appreciable reduction
beyond this point would come dangerously close to the limit of plastic
flow, and consequently an anneal is called for before any further work is
done on the piece.
Figure 13.2.8 shows the approximate true stress vs. true strain plot of
common plastic range values, for comparison with Fig. 13.2.6. In metal
forming, a convenient way of representing the resistance of metal to
Fig. 13.2.7 Graphical solution of a metalworking problem.
Fig. 13.2.5 Testing methods used to determine mechanical behavior of materials under various deformation regimes.
(Source: J. E. Field, W. G. Proud, S. M. Walley, and H. T. Goldrein, Review of Experimental Techniques for High Rate
Deformation and Shock Studies, in “New Experimental Methods in Material Dynamics and Impact,” AMAS, Warsaw, 2001.)
Creep Quasi-static Bar impact
Light gas gun
Strain vs time
creep rate recorded
Inertia forces neglected
Increasing stress levels
Inertia forces important
Characteristic time (s)
Strain rate (s−1
Fig. 13.2.6 Plastic range chart of commonly worked metals.
Section_13.qxd 10/05/06 10:32 Page 13-12
deformation and flow is the flow stress s, also known as the logarithmic
stress or true stress. For most metals, flow stress is a function of the
amount of deformation at cold-working temperatures (strain ) and the
deformation rate at hot-working temperatures (strain rate ) This rela-
tionship is often given as a power-law curve; for cold form-
ing and for hot forming. For commonly used materials, the
values of the strength coefficients K and C and hardening coefficients
n and m are given in Tables 13.2.1a and b.
A practical manufacturing method of judging relative plasticity is to
compute the ratio of initial yield point to the ultimate tensile strength as
developed in the tensile test. Thus a General Motors research memo listed
steel with a 0.51 yield/tensile ratio [22,000 lb/in2
) yp/ 43,000
) ultimate tensile strength] as being suitable for really
severe draws of exposed parts. When the ratio reaches about 0.75, the
steel should be used only for flat parts or possibly those with a bend of
not more than 90Њ. The higher ratios obviously represent a narrowing
range of workability or residual plasticity.
Advanced High-Strength Sheet Steels With greater emphasis being
placed on weight reduction, many new grades of steel sheets for automo-
tive bodies have been developed. Interstitial free (IF) steels were
developed for applications requiring high ductility, BH bake hardening
(BH) steels for dent resistance, dual phase (DP), transformation-induced
plasticity (TRIP), complex phase (CP), and ferritic-bainitic (FB) steels for
high-strength applications such as body panels and pillars (Fig. 13.2.9).
There is a tradeoff between formability and strength in these steels. The
steel industry is trying to develop steel grades that would improve both
these properties simultaneously. For example, DP500, DP600, DP750, and
TRIP800 grades have maximum strengths of 600, 650, 825, and 1,000
MPa, respectively. This is much higher than the 500 MPa expected from
HSLA360, the most common sheet steel for automotive bodies.
Rolling of sheets, coils, bars, and shapes is a primary process using
plastic ranges both above and below recrystallization to prepare metals
for further working or for fabrication. Metal squeezed in the bite area of
s 5 C e
s 5 Ken
the rolls moves out lengthwise with very little spreading in width. This
compressive working above the yield point of the metal may be aided
in some cases by maintaining a substantial tensile strain in the direction
A cast or forged billet or slab is preheated for the preliminary break-
down stage of rolling, although considerable progress has been made in
continuous casting, in which the molten metal is poured continuously
into a mold in which the metal is cooled progressively until it solidifies
(albeit still at high temperature), whence it is drawn off as a quasi-
continuous billet and fed directly into the first roll pass of the rolling mill.
The increased speed of operation and production and the increased effi-
ciency of energy consumption are obvious. Most new mills, especially
minimills, have incorporated continuous casting as the normal method
of operation. A reversing hot mill may achieve 5,000 percent elongation
of an original billet in a series of manual or automatic passes.
Alternatively, the billet may pass progressively through, say, 10 hot mills
in rapid succession. Such a production setup requires precise control so
that each mill stand will run enough faster than the previous one to
Fig. 13.2.8 True stress vs. true strain curves for typical metals. (Crane and Hauf, E. W. Bliss. Co.)
ROLLING OPERATIONS 13-13
Fig. 13.2.9 New high-strength sheet steels for automotive bodies. (Source:
Ultra Light Steel Autobody Consortium, USA.)
Body panels Structural parts
Current state of technology
Section_13.qxd 10/05/06 10:32 Page 13-13
Section_13.qxd 10/05/06 10:32 Page 13-15
13-16 PLASTIC WORKING OF METALS
make up for the elongation of the metal that has taken place. Hot-rolled
steel may be sold for many purposes with the black mill scale on it.
Alternatively, it may be acid-pickled to remove the scale and treated
with oil or lime for corrosion protection. To prevent scale from forming
in hot-rolling, a nonoxidizing atmosphere may be maintained in the mill
area, a highly special plant design.
Pack rolling of a number of sheets stacked together provides means of
retaining enough heat to hot-roll thin sheets, as for high-silicon electric
Cold-rolling is practical in production of thin coil stock with the more
ductile metals. The number of passes or amount of reduction between
anneals is determined by the rate of work hardening of the metal.
Successive stands of cold-rolling help to retain heat generated in work-
ing. Tension provided by mill reels and between stands helps to increase
the practical reduction per step. Bright annealing in a controlled atmos-
phere avoids surface pockmarks, which are difficult to get out. For high-
finish stock, the rolls must be maintained with equal finish.
Cold Rolling of Threads and Gears Threaded parts, mostly fasten-
ers, are cold-rolled with special tooling to impart a typical helical thread
geometry to the part. The thread profile is most often a standard 60Њ vee,
although thread profiles (i.e., Acme) for power threads are possible and
have been produced. In one form, the tooling consists of two tapered rec-
iprocating dies with the desired thread profile cut thereon. A blank of
diameter smaller than the OD of the screw is positioned between the dies
when they are at maximum separation. Then, as the dies reciprocate and
decrease the gap between them, the blank is gripped, rolled, and plasti-
cally deformed to the desired screw profile. The indenting dies displace
metal upward to form the upper part of the thread profile. There is no
waste metal, and the fastener suffers no tears at the root. The resulting
cold work and plastic displacement of metal results in a superior prod-
uct. Subsequent heat treatment of the fastener may follow, depending on
the strength properties desired for a particular application.
Thread rolling is also accomplished by using a nest of three profiled
rotating rollers. In that case, the blank is fed axially when the rollers are
at maximum gap and then is plastically deformed as the roll gap closes
Gear profiles also can be rolled. The action is similar to that described
for rolling threads, except that the dies or rollers are profiled to impart the
desired involute gear profile. The gear blank is caught between the rollers
or dies, and conjugate action ensues between the blank and tooling as the
blank progresses through the operating cycle. In some applications, the
rolled gear is produced slightly oversize to permit a finer finish by subse-
quent hobbing. The advantage lies in the reduction of metal cut by the
hob, thereby increasing the production rate as well as maintaining the
beneficial cold-worked properties imparted to the metal by cold rolling.
Thread and gear rolling enables high production rates; most threaded
fasteners in production are of this type.
Protective coating is best exemplified by high-speed tinplate mills in
which coil stock passes continuously through the necessary series of
cleaning, plating, and heating steps. Zinc and other metals are also
applied by plating but not on the same scale. Clad sheets (high-strength
aluminum alloys with pure aluminum surface for protection against
electrolytic oxidation) are produced by rolling together; an aluminum
alloy billet is hot-rolled together with plates of pure aluminum above
and below it through a series of reducing passes, with precautions to
ensure clean adhesion.
On the other hand, prevention of adhesion, as by a separating film, is
essential in the final stages of foil rolling, where two coils may have to be
rolled together. Such foil may then be laminated with suitable adhesive
to paper backing materials for wrapping purposes. (See also Sec. 6.)
Shape-rolling of structural shapes and rails is usually a hot operation
with roll-pass contours designed to distribute the displacement of metal
in a series of steps dictated largely by experience. Contour rolling of rel-
atively thin stock into tubular, channel, interlocking, or varied special
cross sections is usually done cold in a series of roll stands for length-
wise bending and setting operations. There is also a wide range of sim-
ple bead-rolling, flange-rolling, and seam-rolling operations in
relatively thin materials, especially in connection with the production of
barrels, drums, and other containers.
Oscillating or segmental rolling probably developed first in the manually
fed contour rolling of agricultural implements. In some cases, the suitably
contoured pair of roll inserts or roll dies oscillates before the operator, to
form hot or cold metal. In other cases, the rolls rotate constantly, toward
the operator. The working contour takes only a portion of the circumfer-
ence, so that a substantial clearance angle leaves a space between the rolls.
This permits the operator to insert the blank to the tong grip between the
rolls and against a fixed gage at the back. Then, as rotation continues, the
roll dies grip and form the blank, moving it back to the operator. This
process is sometimes automated; such units as tube-reducing mills oscillate
an entire rolling-mill assembly and feed the work over a mandrel and into
the contoured rolls, advancing it and possibly turning it between recipro-
cating strokes of the roll stands for cold reduction, improved concentricity,
and, if desired, the tapering or forming of special sections.
Spinning operations (Fig. 13.2.10) apply a rolling-point pressure to
relatively limited-lot production of cup, cone, and disk shapes, from
floor lamps and TV tube housings to car wheels and large tank ends.
Where substantial metal thickness is required, powerful machines and
hydraulic servo controls may be used. Some of the large, heavy sections
and difficult metals are spun hot.
Fig. 13.2.10 Spinning operations.
Rolling operations are distinguished by the relatively rapid and con-
tinuous application of working pressure along a limited line of contact.
In determining the working area, consider the lineal dimension (width
of coil), the bite (reduction in thickness), and the roll-face deflection,
which tends to increase the contact area. Approximations of rolling-mill
load and power requirements have been worked out in literature of the
AISE and ASME.
The shearing group of operations includes such power press operations
as blanking, piercing, perforating, shaving, broaching, trimming, slit-
ting, and parting. Shearing operations traverse the entire plastic range
of metals to the point of failure.
The maximum pressure P, in pounds, required in shearing operations
is given by the equation P ϭ pDtS ϭ Lts, where s is the resistance of
the material to shearing, lb/in2
; t is the thickness of the material, in;
L is the length of cut, in, which is the circumference of a round blank
pD or the periphery of a rectangular or irregular blank. Approximate
values of s are given in Table 13.2.2.
Shear (Fig. 13.2.11) is the advance of that portion of the shearing
edge which first comes in contact with the material to be sheared over
the last portion to establish contact, measured in the direction of
motion. It should be a function of the thickness t. Shear reduces the
maximum pressure because, instead of shearing the whole length of cut
Section_13.qxd 10/05/06 10:32 Page 13-16
at once, the shearing action takes place progressively, shearing at only
a portion of the length at any instant. The maximum pressure for any
case where the shear is equal to or greater than t is given by Pmax ϭ
Pav t/shear, where Pav is the average value of the pressure on a punch,
with shear ϭ t, from the time it strikes the metal to the time it leaves.
Distortion results from shearing at an angle (Fig. 13.2.11) and accord-
ingly, in blanking, where the blank should be flat, the punch should be
flat, and the shear should be on the die. Conversely, in hole punching,
where the scrap is punched out, the die should be flat and the shear
should be on the punch. Where there are a number of punches, the effect
of shear may be obtained by stepping the punches.
Crowding results during the plastic deformation period, before the
fracture occurs, in any shearing operation. Accordingly, when small
delicate punches are close to a large punch, they should be stepped
shorter than the large punch by at least a third of the metal thickness.
Clearance between the punch and die is required for a clean cut and
durability. An old rule of thumb places the clearance all around the
punch at 8 to 10 percent of the metal thickness for soft metal and up to
12 percent for hard metal. Actually, hard metal requires less clearance
for a clean fracture than soft, but it will stand more. In some cases, with
delicate punches, clearance is as high as 25 percent. Where the hole
diameter is important, the punch should be the desired diameter and the
clearance should be added to the die diameter. Conversely, where the
blank size is important, the die and blank dimensions are the same and
clearance is deducted from the punch dimensions.
The work per stroke may be approximated as the product of the maxi-
mum pressure and the metal thickness, although it is only about 20 to
80 percent of that product, depending upon the clearance and ductility
of the metal. Reducing the clearance causes secondary fractures and
increases the work done. With sufficient clearance for a clean fracture,
the work is a little less than the product of the maximum pressure, the
metal thickness, and the percentage reduction in thickness at which the
fracture occurs. Approximate values for this are given in Table 13.2.2.
The power required may be obtained from the work per stroke plus a 10
to 20 percent friction allowance.
Shaving A sheared edge may be squared up roughly by shaving
once, allowing for the shaving of mild sheet steel about 10 percent of the
metal thickness. This allowance may be increased somewhat for thinner
material and should be decreased for thicker and softer material. In mak-
ing several cuts, the amount removed is reduced each time. For extremely
fine finish a round-edged burnishing die or punch, say 0.001 or 0.0015
in tight, may be used. Aluminum parts may be blanked (as for impact
extrusion) with a fine finish by putting a 30Њ bevel, approx one-third the
metal thickness on the die opening, with a near metal-to-metal fit on the
punch and die, and pushing the blank through the highly polished die.
Squaring shears for sheet or plate may have their blades arranged in
either of the ways shown in Fig. 13.2.12. The square-edged blades in
Fig. 13.2.12a may be reversed to give four cutting edges before they are
reground. Single-edged blades, as shown in Fig. 13.2.12b, may have a
clearance angle on the side where the blades pass, to reduce the work-
ing friction. They may also be ground at an angle or rake, on the face
which comes in contact with the metal. This reduces the bending and
consequent distortion at the edge. Either type of blade distorts also in
the other direction owing to the angle of shear on the length of the
blades (see Fig. 13.2.11).
Circular cutters for slitters and circle shears may also be square-edged
(on most slitters) or knife-edged (on circle shears). According to one rule,
their diameter should be not less than 70 times the metal thickness.
Knife-edge hollow cutters working against end-grain maple blocks rep-
resent an old practice in cutting leather, rubber, and cloth in multiple
thicknesses. Steel-rule dies, made up of knife-edge hard-steel strip
economically mounted against a steel plate in a wood matrix with rubber
Table 13.2.2 Approximate Resistance to Shearing in Dies
Annealed state Hard, cold-worked
Resistance Penetration Resistance Penetration
to shearing, to fracture, to shearing, to fracture,
* percent lb/in2
Lead 3,500 50 Anneals at room temperature
Tin 5,000 40 Anneals at room temperature
Aluminum 2S, 3S 9,000–11,000 60 13,000–16,000 30
Aluminum 52S, 61S, 62S 12,000–18,000 . . . 24,000–30,000
Aluminum 75S 22,000 . . . 46,000
Zinc 14,000 50 19,000 25
Copper 22,000 55 28,000 30
Brass 33,000–35,000 50–55 52,000 25–30
Bronze 90–10 . . . . . . 40,000
Tobin bronze 36,000 25 42,000
Steel 0.10C 35,000 50 43,000 38
Steel 0.20C 44,000 40 55,000 28
Steel 0.30C 52,000 33 67,000 22
Steel 0.40C 62,000 27 78,000 17
Steel 0.60C 80,000 20 102,000 9
Steel 0.80C 97,000 15 127,000 5
Steel 1.00C 115,000 10 150,000 2
Stainless steel 57,000 39
Silicon steel 65,000 30
Nickel 35,000 55
ϭ 6.895 MN/m2
NOTE: Available test data do not agree closely. The above table is subject to verification with closer control of metal analysis,
rolling and annealing conditions, and die clearances. In dinking dies, steel-rule dies, hollow cutters, etc., cutting-edge resistance is
substantially independent of thickness: cotton glove cloth (stack, 2 or 3 in thick), 240 lb/in; kraft paper (stack tested, 0.20 in thick),
385 lb/in, celluloid [ in thick, warmed in water to 120 to 150ЊF (49 to 66ЊC)], 300 lb/in.11⁄32
Fig. 13.2.11 Shearing forces can be reduced by providing a rake or shear on
(a) the blades in a guillotine, (b) the die in blanking, (c) the punch in piercing.
(J. Schey, “Introduction to Manufacturing Processes,” McGraw-Hill, 1987.)
Section_13.qxd 10/05/06 10:32 Page 13-17